The shear bond strength of reconditioned sapphire bracket
after rebonding with sandblasting zirconia
Dedeh Pitriani*, Setiadi W. Logamarta*, Dian N. Agus Imam*
*Department of Orthodontics Faculty of Dentistry Jenderal Soedirman University, Indonesia
Introduction: Sapphire bracket is the best aesthetic bracket with metal bracket-like mechanical properties. In conditions causing attachment lost between sapphire bracket and enamel, a rebonding procedure will needed. The shear bond strength of sapphire bracket decrease after the rebonding
procedure. Sandblasting, hydroluoric acid etching, and silanization as surface treatment are widely used to improve the bracket bond strength. The purpose of this study was to evaluate the efect of zirconia
as sandblasting material towards the shear bond strength of reconditioned sapphire bracket. Methods:
This study was an experimental laboratory with as much as 27 samples of sapphire bracket divided into 3
groups. Group I was rebonded with sandblasting zirconia and silane, group II with hydroluoric acid etching
and silane, and group III with new bracket bonding. The attachment strength measurement indicator was the shear bond strength test and the SEM analysis. Results: The shear bond strength test showed the average value for each group were 12.97 MPa, 9.26 MPa, and 10.58 MPa, consecutively. The test results
were then analysed using a one way ANOVA and LSD (p < 0.05), which showed that signiicant diference
only found in the comparison between group I with group II, but not in the comparison between group I with group III. The SEM analysis result showed that sandblasted surface has homogenous microporosities in high quantities. Conclusion: Zirconia as sandblasting material was efective in increasing the shear bond strength of reconditioned sapphire bracket.
Keywords: Sandblasting, sapphire bracket, shear bond strength, zirconia.
Corresponding author: Dedeh Pitriani, Department of Orthodontics Faculty of Dentistry Jenderal Soedirman University Dr. Soeparno St., Karawangkal Campus Building E, Banyumas, Central Java 53122. e-mail: firstname.lastname@example.org INTRODUCTION
The sapphire bracket is a type of ceramic bracket that has the best aesthetic value and mechanical properties equivalent to a metal bracket. Another advantage of the sapphire bracket is the colour stability, non-toxic, corrosion resistant, and
biocompatible.1 Conditions such as overly heavy chewing loads, tooth brushing processes that are too hard or deliberately removed due to debonding procedures, cause attachment between brackets and emails are released, so a re-attachment procedure is required.2 Strong adhesive sliding sapphire bracket decreases when re-attached
p-ISSN 1979-0201, e-ISSN 2549-6212 Available from: http://jurnal.unpad.ac.id/pjd/article/view/13602
because the surface of the sapphire bracket base is distorted due to debonding procedure or cleaning of adhesive residue. The addition of retention is required for the shear strength of shear to increase, for example sandblasting.3
Sandblasting is performed by iring abrasive
material at a certain distance and pressure, which will clean up the remaining adhesive material and produce a new microporosity as mechanical retention.4 Materials commonly used as materials sandblasting in dentistry is aluminium oxide. Aluminium oxide is a ceramic material that has a high hardness but has brittle properties that easily break. These particles are shown to increase surface roughness and mechanical bonding.
Technological developments in natural resource processing, encouraging innovation by utilising local resources as raw materials. One of
Indonesia’s potential resources is zirconia. Zirconia
is a mineral that is widely available in Indonesia, especially in Bangka and Kalimantan.6 Zirconia has a density of 6.42 g/cm3, high strength, high fracture resistance, high hardness, and resistant to acid and base corrosion. In addition to these
properties, zirconia has excellent biocompatibility
and is quite aesthetic.7
Zirconia is widely used in the ield of
dentistry such as the manufacture of denture.8 Zirconia can be used as an abrasive material because it can maintain its particle shape. Zirconia can be used as an additional material to improve the mechanical properties of the material.7 One
of them is a zirconate coupling agent that helps
the non-silica ceramic adhesion.9
Background above, encouraging researchers
to see the efect of the use of zirconia as a
sandblasting material against the shear bonding strength of reconditioning the base of the sapphire bracket. A scanning electron microscopy (SEM) test was used to assess surface morphology after sandblasting, and a shear bond strength test was
used to measure the efectiveness of the bracket
The type of research conducted was a pure laboratory experimental research with post test only control group design. The research was conducted at the Basic Dentistry Laboratory of
Jenderal Soedirman University. The number of samples in this study was 27 samples divided into three treatment groups. The materials used in this study were American Orthodontics® Radiance Plus
sneak bracket, mandibular irst premolar teeth, light cure adhesive bonding, zirconia, cold acrylic resin, 9% hydroluoric acid, 37% phosphoric acid,
The research procedures were as follows: 1) Sample preparation: Acrylic prints are 13 mm in diameter and 7 mm in height. The maxillary premolar teeth were cut to 1 mm below the cementoenamel junction with the diamond of the bur disk and the cervical section covered in the night. The teeth were grown on acrylic with the buccal surface facing upwards. The sample picture can be seen in Figure 1 below.
The enamel particles were cleaned with pumice and water then etched with 37% phosphoric acid for 30 seconds, rinsed with running water for 10 seconds and dry. Afterwards, the bonding material was applied, the bracket was sticked to the buccal portion of the tooth with the bracket slot to the 4 mm cups. The bracket then pressed
with 4 oz force gauge or 113.4 g for 10 seconds.
Irradiation was performed for 40 seconds with
intensity 1000 mW / cm2, incubated in an artiicial
saliva solution, temperature 37ºC for 24 hours. The bonding treatment was performed by fully polymerised the bonding material, then the
Figure 1. Sample mould
Figure 2. Sample mould II
Acrylic resin was poured into mould II
Table 1. The mean and standard deviation of sapphire brackte shear bond strength
Sandblasting zirconia (MPa)
Etsa 9% Hydroluoric acid etch (MPa) New Bonding (MPa)Group III
Mean 12.97 9.26 10.58
SD 3.12 2.92 2.20
bracket was debonded to the tooth surface using a debonding plier. The technique used was the
squeeze, both ends of pliers pressed on mesial and
distal wings. Treatment in group I was performed by cleaning the remaining adhesive material with tungsten carbide round bur for 32 seconds, then
the sandblasting procedure of 25 μm zirconia for
30 seconds with a pressure of 2.3 bar and 900 angles. Treatment in group II was performed by cleaning the remaining adhesive material with tungsten carbide round bur for 32 seconds, then
etched with 9% hydroluoric acid for 20 seconds
and rinsed with water. Treatment in Group III, no debonding procedure and re-attachment was performed. Scanning electron microscopy (SEM) test was performed after the surface treatment process, one sample from each group was not being rebonded. The sample was analysed by SEM to see the surface microporosity and to know the
residual zirconia on the surface of the sapphire
The rebonding procedure was performed by cleaning the rest of the adhesive material on the buccal surface of the tooth with green stone bur low speed or scaler and pumice and water. The base of the bracket base was added with silane using a micro brush and repeated the bonding procedure. The sample on an uncoupled mould I was coated with vaseline. The second mould was placed over the sample, and the acrylic resin was manipulated and then loaded into the mould II. The description of the mould II can be seen in Figure 2 below.
Shear bond strength testing was performed towards reinstalled brackets using the universal testing machine. The results obtained in the form of load or shear force (F) in units of Newton (N). The data, included in the shear strength formula
τ = F / A with τ = shear strength (MPa), F = shear force (N), and A = bracket base area (mm2).
Data analysis was performed to see the normality of data using Shapiro Wilk test and see the homogeneity of data with the Shapiro-Wilk
test. Furthermore, the parametric statistical test was performed in the form of one way ANOVA. One way ANOVA tested the hypothesis with one dependent variable. Then, followed by Post Hoc
Least Signiicant Diference (LSD) analysis with 95% conidence level (α = 0.05) to see a signiicant diference between sample groups.
Test results of the shear bond strength using the universal testing machine tool was performed to see the shear bond strength of each group. The average value of the shear bond strength value can be seen in Table 1.
Figure 3 showed group I having the highest mean and group II having the lowest mean value. The data were tested for normality using Shapiro-wilk test with a p-value higher than 0.05, showing normal distribution data. Normality test results can be seen in Table 2.
Table 2 showed that the normality test values use the Shapiro-wilk test. This test showed that the p-value of the whole group was higher than 0.05, so the data was normally distributed. Data was tested the homogeneity using Levene test with p-value more than 0,05 indicating the data homogeneous. Homogeneity test results can be seen in Table 3.
Statistic Sample number p
Shear bond strength
I 0.965 8 0.853
II 0.910 8 0.351
III 0.914 8 0.386
Table 2. Shapiro-wilk normality data test of sapphire bracket shear bond strength
Levene statistic df1 df2 p
0.968 2 21 0.396
Table 3. Levene homogeinity test result of sapphire bracket shear bond strength
Groups df Variances f p
Between groups 2 28.36
Inside group 21 7.73
Table 4. One-way ANOVA statistic test result of the mean value of sapphire bracket shear bond strength
Table 5. LSD statistic test result of the mean value of sapphire bracket shear bond strength
Group I Group II Group III
Group I 0.014* 0.099
Group II 0.014* 0.355
Group III 0.099 0.355
Figure 5. Description of the SEM results of 2000 x magniication. (A) Group I; (B) Group II; (c) Group III Figure 4. Description of the SEM results of 1000 x magniication. (A) Group I; (B) Group II; (c) Group III. The showed microporosity; the showed adhesive material residue; the showed zirconia particles residue; the
showed new retention formation on the new bracket
Table 3 showed the homogeneity test values using Levene test. This test showed that the p-value of the whole group was higher than 0.05, so the data was homogeneous. Furthermore, one way ANOVA test was performed to determine the
diferences between groups. The test results can
be seen in Table 4.
From the test results can be concluded
that there was a signiicant diference of the
mean value of the shear bond strength between
all research groups. The post-hoc least signiicant diference (LSD) test was performed to determine the signiicance of the diferences in each group. The data was considered of having signiicant diferences if the value of p < 0.05. LSD test
results can be seen in Table 5.
Group I and group II had signiicant diferences with the p-value of 0.014. Group I and group III did not have signiicant diferences,
with the p-value of 0.099, and group III with
group II did not show any signiicant diference with the p-value of 0.355. After 9% hydroluoric
bracket base. SEM description of groups 1 and
group 2 with magniication 1000x and 2000x can
be seen in Figure 4 and Figure 5.
Microporosity was observed more in Group
I, and the size tends to be more similar. Around
the microporosity was observed white particles
with various sizes which were the zirconia
sandblasting residue. Group II was seen as having
less microporosity, and the size tends to be
less homogenous than group I. Group III showed undercut retention.
Analysis of the shear bond strength of reconditioned sapphire bracket was presented in Table 1. The
re-attachment with sandblasting zirconia plus silane
treatment has the highest shear bond strength.
One reason was that the zirconia particles being ired were able to heat the bracket base surface,
resulting in the formation of a new microporosity that acted as micromechanical retention, as well as removing the remaining adhesive material on the undercut.
Figure 2 showed the microporosity
generated by a large number of zirconia
sandblasting procedures with uniformly inclined
sizes. A large number of microporosities of uniform size automatically create a more formed
micromechanical interlocking and tend to have similar strength across the surface, resulting in stronger attachment, and increased shear strength increasing. The remaining adhesive material in
group I was less than group II. Sandblasting zirconia efectively removes the remaining adhesive
material on a bracket base. Optimal cleansing makes micromechanical interlocking between the adhesive material and the undercut stronger, thereby increasing the strength of retractable shear. The ability to clean up the rest of the adhesive material and form a new microporosity is what makes the micromechanical interlocking in group I to be increased. The results of this study were in accordance with previous research which stated that the sandblasting procedure
was efective to clean the surface of the bracket
base and increase the strength of ceramic bracket attachment.10
The area around the microporosity was a
white particle of various sizes which is zirconia
attached to the base of the bracket base and can be an instrument to enhance attachment. Zirconia particles have a large adsorption capacity against phosphate groups silane, the phosphoric methacrylate. Zirconia combined with phosphate groups will have an active surface and a high
chemical ainity, thereby increasing attachment
strength. Prior research suggests that increased attachment strength was obtained by bonding between phosphate monomers in lutting materials
and zirconia surfaces.11
In addition to reacting with zirconia
particles, the functional group on the silane would bind to the organic material on the adhesive material, and the inorganic material in the silane was able to bind with the sapphire bracket to form a siloxane (Si-O-Si) bond. The bond would increase the resin cement attachment by bracketing chemically, thereby increasing the shear strength of shear in group I. This result was in accordance with previous research stated that silane in bracket re-attachment procedure could provide adequate shear strength.2
Table 2 showed the second group of
reactor-treated groups with 9% hydroluoric acid etching
application plus silane having the lowest average shear bond strength. This condition may occur because the microporosity was formed less with
more varied size. Consequently, micromechanical
interlocking is formed less with less stable power, so the shear bond strength of attachment tends to be less than the maximum, and this makes the average strong shear adhesive in group II to the lowest.
The etching may dissolve the debris on the surface of the bracket base, in Figure 5 of the base surface of the bracket after cleaner etching. This condition will increase the surface energy so that it can optimise the bond between the silane with adhesive and bracket. The bond formed is a siloxane bond (Si-O-Si), which was the functional group on the silane binds with the adhesive material, and the inorganic group binds to the bracket. Thus, despite the low shear bond strength of group II, it still achieved a clinically acceptable standard of 6-8 MPa.
The LSD test in Table 4 showed signiicant diferences between group I and group II. This result was inluenced by the pattern of
to be uniform, the remaining adhesive material of group I is less than group II, and the remaining
part of zirconia particles left in group I so that the
average of shear bond strength was higher than Group II.
Table 1 showed that group III of the new rebonded bracket had a higher mean value than Group II but lower than Group I. The attachment to the new bracket was obtained by the mechanical bond between the bracket and the adhesive material. The surface of the bracket base in Group III has mechanical retention of the undercut, resulting in an adequate micromechanical interlocking between the bracket and the adhesive material. The result obtained was the optimal shear strength of the bracket attachment.
The LSD test between group III and group
I showed no signiicant diference. This condition
showed that the procedure of re-attachment with
sandblasting zirconia method was able to produce the shear that is not much diferent from new attachment. Sandblasting with zirconia can clean
the residual adhesive material on the surface of the bracket base while forming a microporosity that serves as mechanical retention.
Bonding between silanes with sandblasting particles and adhesive materials are able to help improve attachment strength. Therefore, the shear bond strength of produced by group I was equivalent to a new attachment bracket. The results of previous studies stated that the rebonded ceramic bracket by the sandblasting procedure had a shear bond strength comparable to the new attachment.12 The rebonded procedure with sandblasting plus silane yields high shear strength and the equivalent of a new bracket attachment strength.2
The SEM image showed the surface of the rebounded sapphire bracket base after the
sandblasting procedure using zirconia to have
more microporosity and a uniformly inclined shape. This result was caused due to the microporosity formation mechanically through
zirconia particles that were ired at a certain
pressure and duration, thus causing friction between the sandblasting particles with the bracket base. Friction between particles causes the surface to become hot and melt, resulting in the formation of microporosity. More sandblasting
microporosity patterns of this uniform size tend to
cause micromechanical interlocking to increase. Microporosity pattern in group II was formed
from chemical activity, namely hydroluoric acid
which dissolved the structure in the ceramic to form microporosity and looks like there was an open structure. The interaction between
hydroluoric acid and silica partly forms insoluble hexaluorosilicate, and the other half dissolves
the silica. As a result, the crystalline structure is open, and microporosity is formed. Such conditions can increase the surface energy, and the addition
of silanes will increase the efectiveness of
attachment. The resulting microporosity was less,
the efectiveness of attachment decreases, hence
the lowest shear strength compared to the other groups.
Zirconia as sandblasting material was efective in
increasing the shear bond strength of reconditioned sapphire bracket.
1. Brantley WA, Eliades T. Orthodontic
material-scientiic and clinical Aspects. New York:
Thieme Stuttgart. 2001.
2. Falkensammer F, Jonke E, Bertl M, Freudentahler J, Bentleon HP. Rebonding
performance of diferent ceramic brackets
conditioned with a new silane coupling agent. Eur J Orthod 2013;35:103-9.
3. Jena K, Duggal R, Mehrotra AK. Physical properties and clinical characteristics of ceramic bracket: A comprehensive review. Trends Biomater 2007;20(2):138-41.
4. Chetan GB, Muralidhar RY. Comparative
evaluation of four oice reconditioning
methods for orthodontic stainless steel bracket on shear bond strenth: An In Vitro Study. Essences Dentistry 2011;3:6-13.
5. Andrade PHR, Reges RV, Lenza MA. Evaluation
of shear bond strength of diferent treatments
of ceramic bracket surfaces. Dental Press J Orthod 2012;17(4):17el-8. DOI:10.22159/ ijap.2017.v9s2.16
6. Sudjoko D, Triyono. Peningkatan kualitas
zirkonia hasil olahan pasir zirkon. Ganendra
7. Christache CM, Burlibasa M, Cristache G, Drafta S, Popovici A, Iliescu AA, et al. Zirconia and its biomedical application. Metalurgia International 2011;16(7):18-23.
8. Saridag S, Tak O, Alniacik G. Basic properties
and type of zirconia : An overview. World J
9. Thompson JY, Stoner BR, Piascik JR, Smith R.
Adhesion/cementation to zirconia and other
non-silicate ceramics: What are we now?. Dent Mater 2011;27(1):71-82. DOI:10.1016/j. dental.2010.10.022.
10. Guarita MK, Moresca AH, Losso EM, Moro A,
Moresca RC, Correr GM. Efect of diferent
surface treatment for ceramics bracket base
on bond strength of rebonded brackets. Braz
Dent J 2015;26(1):61-5. DOI:10.1590/0103-6440201300234.
11. Nishigawa G, Maruo Y, Irie M, Maeda N,
Yoshihara K, Nagaoka N, et al. Various efect of sandblasting of dental restorative
materials. Plos One Journal. 2016;11(1):1-10. DOI:10.1371/0147077.
12. Al Maaitah EF, Alomari S, Alhaija SAA, Sai
AA. The efect of diferent bracet base